| ||Format||Pages||Price|| |
|16||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||16||$50.00||  ADD TO CART|
Significance and Use
5.1 Fracture mirror size analysis is a powerful tool for analyzing glass and ceramic fractures. Fracture mirrors are telltale fractographic markings in brittle materials that surround a fracture origin as discussed in Practices and . shows a schematic with key features identified. shows an example in glass. The fracture mirror region is very smooth and highly reflective in glasses, hence the name “fracture mirror.” In fact, high magnification microscopy reveals that, even within the mirror region in glasses, there are very fine features and escalating roughness as the crack advances away from the origin. These are submicrometer in size and hence are not discernable with an optical microscope. Early investigators interpreted fracture mirrors as having discrete boundaries including a “mirror-mist” boundary and also a “mist-hackle” boundary in glasses. These were also termed “inner mirror” or “outer mirror” boundaries, respectively. It is now known that there are no discrete boundaries corresponding to specific changes in the fractographic features. Surface roughness increases gradually from well within the fracture mirror to beyond the apparent boundaries. The boundaries were a matter of interpretation, the resolving power of the microscope, and the mode of viewing. In very weak specimens, the mirror may be larger than the specimen or component and the boundaries will not be present.
5.5 A, the “fracture mirror constant” (sometimes also known as the “mirror constant”) has units of stress intensity (MPa√m or ksi√in) and is considered by many to be a material property. As shown in , it is possible to discern separate mist and hackle regions and the apparent boundaries between them in glasses. Each has a corresponding mirror constant, A. The most common notation is to refer to the mirror-mist boundary as the inner mirror boundary, and its mirror constant is designated Ai. The mist-hackle boundary is referred to as the outer mirror boundary, and its mirror constant is designated Ao. The mirror-mist boundary is usually not perceivable in polycrystalline ceramics. Usually, only the mirror-hackle boundary is measured and only an Ao for the mirror-hackle boundary is calculated. A more fundamental relationship than may be based on the stress intensity factors (KI) at the mirror-mist or mist-hackle boundaries, but is more practical and simpler to use.
5.6 The size predictions based on and the A values, or alternatively stress intensity factors, match very closely for the limiting cases of small mirrors in tension specimens. This is also true for small semicircular mirrors centered on surface flaws in strong flexure specimens. So, at least for some special mirror cases, A should be directly related to a more fundamental parameter based on stress intensity factors.
5.7 The size of the fracture mirrors in laboratory test specimen fractures may be used in conjunction with known fracture mirror constants to verify the stress at fracture was as expected. The fracture mirror sizes and known stresses from laboratory test specimens may also be used to compute fracture mirror constants, A.
5.8 The size of the fracture mirrors in components may be used in conjunction with known fracture mirror constants to estimate the stress in the component at the origin. Practice has a comprehensive list of fracture mirror constants for a variety of ceramics and glasses.
1.1 This practice pertains to the analysis and interpretation of fracture mirror sizes in brittle materials. Fracture mirrors ( ) are telltale fractographic markings that surround a fracture origin in brittle materials. The fracture mirror size may be used with known fracture mirror constants to estimate the stress in a fractured component. Alternatively, the fracture mirror size may be used in conjunction with known stresses in test specimens to calculate fracture mirror constants. The practice is applicable to glasses and polycrystalline ceramic laboratory test specimens as well as fractured components. The analysis and interpretation procedures for glasses and ceramics are similar, but they are not identical. Different optical microscopy examination techniques are listed and described, including observation angles, illumination methods, appropriate magnification, and measurement protocols. Guidance is given for calculating a fracture mirror constant and for interpreting the fracture mirror size and shape for both circular and noncircular mirrors including stress gradients, geometrical effects, and/or residual stresses. The practice provides figures and micrographs illustrating the different types of features commonly observed in and measurement techniques used for the fracture mirrors of glasses and polycrystalline ceramics.
Note 1: The initial flaw may grow stably to size ac prior to unstable fracture when the stress intensity reaches KIc. The mirror-mist radius is Ri, the mist-hackle radius is Ro, and the branching distance is Rb. These transitions correspond to the mirror constants, Ai, Ao, and Ab, respectively.
1.2 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C1145 Terminology of Advanced Ceramics
C1256 Practice for Interpreting Glass Fracture Surface Features
C1322 Practice for Fractography and Characterization of Fracture Origins in Advanced Ceramics
ICS Number Code 81.060.20 (Ceramic products)
ASTM C1678-10(2015), Standard Practice for Fractographic Analysis of Fracture Mirror Sizes in Ceramics and Glasses, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top